rdf-syntax-grammar
mods:
  schema location: http://www.loc.gov/mods/v3 http://www.loc.gov/standards/mods/v3/mods-3-2.xsd
  title info:
    title: Grain refinement of cast niobium via equal channel angular extrusion/annealing
  name:
    name part: Bryant, Don O.
    name part: 1960-
    role:
      role term: creator
  name:
    name part: Hartwig, Karl Theodore
    role:
      role term: thesis advisor.
  type of resource: text
  genre: bibliography
  origin info:
    place:
      place term: txu
    date issued: 2007
    issuance: monographic
  language:
    language term: eng
  physical description:
    form: electronic
    form: remote
  abstract: This research investigated the effectiveness of equal channel angular extrusion (ECAE) and annealing to improve the grain morphology and mechanical properties of electron-beam remelted pure niobium. Extrusions were performed at room temperature with a 90° die. Routes 1A, 2C, 4E and 8E were investigated with duplicate billets undergoing routes 1A, 2C and 4E to determine reproducibility. Niobium proved to be very workable during the ECAE process. Hardness increased most dramatically after the first pass and leveled off thereafter. Recrystallization temperatures for the Reference Metals material ranged from a low of 800°C for routes 2C, 4E and 8E to a high of 1000°C for route 1A. For the Wah Chang material, the recrystallization temperatures ranged from a low of 800°C for the 4E ECAE processed material to a high of 950°C for the as received material. The initial grain size and orientation have been hypothesized to be influential on recrystallized grain morphology for ECAE/annealing processed niobium. Smaller initial grains produce a smaller and more homogeneous recrystallized grain microstructure. The average grain diameters for the recrystallized 4EECAE processed Wah Chang material are 13 ± 6.3 mm for the 1000°C annealed state (no banding) and are 21 ± 9.5 [mu]m for the 1100°C annealed state (no banding). Reference Metals material that underwent route 4Eand annealed at 1000°C resulted in an average grain diameter of 28 [mu]m for billet 2 (banding) and an average grain diameter of 32 [mu]m for billet 19 (slight banding). Reference Metals material that underwent route 8E (no banding) annealed at 1000°C resulted in an average grain diameter of 36 [mu]m. Reference Metals material that underwent route 4E samples annealed at 1100°C resulted in an average grain diameter of 26 mm for billet 2(banding) and an average grain diameter of 43 mm for billet 19 (slight banding). Route 8E (significant banding) annealed at 1100°C resulted in an average grain diameter of 29 [mu]m. Strai…
  note: by Don O Bryant.
  note: "Major Subject: Mechanical Engineering"
  note: Title from author supplied metadata (automated record created on Apr. 27, 2007.)
  note: Vita.
  note: Abstract.
  note: Electronic resource.
  note: Mode of access: World Wide Web.
  note: System requirements: World Wide Web access and Adobe Acrobat Reader.
  note: M. S. Texas A&M University 2005.
  note: Includes bibliographical references.
  note: Text (Thesis).
  subject:
    topic: Major mechanical engineering
  subject:
    topic: ECAE
  subject:
    topic: Niobium
  identifier: http://hdl.handle.net/1969.1/4771
  record info:
    record content source: TXA
    record creation date: 070504
    record change date: 20151104192151.0
    record identifier: in00002241345